F Schubert Room temperature properties of semiconductors IIIV arsenides Quantity Symbol AlAs GaAs InAs Unit Crystal structure Z Z Z Gap Direct Indirect I D D Lattice constant 56611 56533 60584 Ban ID: 35091 Download Pdf

149K - views

Published bymarina-yarberry

F Schubert Room temperature properties of semiconductors IIIV arsenides Quantity Symbol AlAs GaAs InAs Unit Crystal structure Z Z Z Gap Direct Indirect I D D Lattice constant 56611 56533 60584 Ban

Download Pdf

Download Pdf - The PPT/PDF document "E F Schubert Room temperature properties..." is the property of its rightful owner. Permission is granted to download and print the materials on this web site for personal, non-commercial use only, and to display it on your personal computer provided you do not modify the materials and that you retain all copyright notices contained in the materials. By downloading content from our website, you accept the terms of this agreement.

Page 1

© E. F. Schubert Room temperature properties of semiconductors: III–V arsenides Quantity Symbol AlAs GaAs InAs (Unit) Crystal structure Z Z Z Gap: Direct ( ) / Indirect ( ) I D D Lattice constant = 5.6611 5.6533 6.0584 Å Bandgap energy = 2.168 1.42 0.354 eV Intrinsic carrier concentration = 10 2 10 7.8 10 14 cm –3 Effective DOS at CB edge = 1.5 10 19 4.4 10 17 8.3 10 16 cm –3 Effective DOS at VB edge = 1.7 10 19 7.7 10 18 6.4 10 18 cm –3 Electron mobility = 200 8500 33,000 cm /Vs Hole mobility = 100 400 450 cm /Vs Electron diffusion constant = 5.2 220 858 cm / s Hole diffusion

constant = 2.6 10 12 cm / s Electron affinity = 3.50 4.07 4.9 V Minority carrier lifetime = 10 –7 10 –8 10 –8 s Electron effective mass * = 0.146 0.067 0.022 Heavy hole effective mass hh * = 0.76 0.45 0.40 Relative dielectric constant = 10.1 13.1 15.1 Refractive index near = 3.2 3.4 3.5 Absorption coefficient near = 10 10 10 cm –1 D = Diamond. Z = Zincblende. W = Wurtzite. DOS = Dens ity of states. VB = Valence band. CB = Conduction band The Einstein relation relates the diffusion constant and mobility in a non-degenerately doped semiconductor: = ( k T / ) Minority carrier diffusion lengths

are given by = ( 1/2 and = ( 1/2 The mobilities and diffusion constants apply to low doping concentrations ( 10 15 cm –3 ). As the doping concentration increases, mobilities and diffusion constants decrease. The minority carrier lifetime applies to doping concentrations of 10 18 cm –3 . For other doping concentrations, the lifetime is given by = –1 ( + –1 , where GaAs = 10 –10 cm /s.

Â© 2020 docslides.com Inc.

All rights reserved.